#------------------------------------------------------------------------------
#$Date: 2020-10-06 11:00:32 +0300 (Tue, 06 Oct 2020) $
#$Revision: 257476 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/97/7239741.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7239741
loop_
_publ_author_name
'Usman, Mohammad'
'Smith, Mark D.'
'Kocevski, Vancho'
'Besmann, Theodore'
'zur Loye, Hans-Conrad'
_publ_section_title
;
 Complex cobalt silicates and germanates crystallizing in a porous
 three-dimensional framework structure
;
_journal_issue                   6
_journal_name_full               CrystEngComm
_journal_page_first              1112
_journal_page_last               1119
_journal_paper_doi               10.1039/C9CE01662G
_journal_volume                  22
_journal_year                    2020
_chemical_formula_moiety         'Co0.50 Cs O4 Si1.50'
_chemical_formula_sum            'Co0.5 Cs O4 Si1.5'
_chemical_formula_weight         268.51
_space_group_crystal_system      monoclinic
_space_group_IT_number           8
_space_group_name_Hall           'I -2y'
_space_group_name_H-M_alt        'I 1 m 1'
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2019-03-22 deposited with the CCDC.	2020-01-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 91.5928(18)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.9926(4)
_cell_length_b                   5.4599(2)
_cell_length_c                   9.3958(6)
_cell_measurement_reflns_used    4385
_cell_measurement_temperature    301(2)
_cell_measurement_theta_max      28.252
_cell_measurement_theta_min      3.093
_cell_volume                     461.14(4)
_computing_cell_refinement       'SAINT Version 8.38a (Bruker, 2016)'
_computing_data_collection       'Bruker APEX3 v2016.5-0 (Bruker, 2016)'
_computing_data_reduction        'SAINT Version 8.38a (Bruker, 2016)'
_computing_molecular_graphics    various
_computing_publication_material  various
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      301(2)
_diffrn_detector_area_resol_mean 10.4
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker D8 QUEST'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0327
_diffrn_reflns_av_unetI/netI     0.0216
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            7199
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        28.294
_diffrn_reflns_theta_max         28.294
_diffrn_reflns_theta_min         3.093
_diffrn_source                   'microfocus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    10.045
_exptl_absorpt_correction_T_max  0.2627
_exptl_absorpt_correction_T_min  0.1934
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2016/2 (Bruker, 2016)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    3.868
_exptl_crystal_description       plate
_exptl_crystal_F_000             486
_exptl_crystal_size_max          0.060
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.020
_refine_diff_density_max         0.757
_refine_diff_density_min         -0.556
_refine_diff_density_rms         0.135
_refine_ls_abs_structure_details
; 
 Refined as an inversion twin. 
;
_refine_ls_abs_structure_Flack   0.50(7)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.150
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     85
_refine_ls_number_reflns         1254
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.149
_refine_ls_R_factor_all          0.0264
_refine_ls_R_factor_gt           0.0209
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0102P)²+2.9428P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0428
_refine_ls_wR_factor_ref         0.0457
_reflns_Friedel_coverage         0.990
_reflns_Friedel_fraction_full    0.995
_reflns_Friedel_fraction_max     0.995
_reflns_number_gt                1141
_reflns_number_total             1254
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c9ce01662g2.cif
_cod_data_source_block           mus1110a
_cod_depositor_comments
;Adding full bibliography for 7239740--7239743.cif.

 Adding full bibliography for 7239740--7239743.cif.
;
_cod_original_sg_symbol_H-M      'I m'
_cod_original_formula_sum        'Co0.50 Cs O4 Si1.50'
_cod_database_code               7239741
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;
_shelx_estimated_absorpt_t_min   0.584
_shelx_estimated_absorpt_t_max   0.824
loop_
_space_group_symop_operation_xyz
'x, y, z'
'x, -y, z'
'x+1/2, y+1/2, z+1/2'
'x+1/2, -y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Cs1 Cs 0.19149(8) 0.000000 0.50822(8) 0.0292(4) Uani 1 2 d S T P
Cs2 Cs 0.71441(7) 0.000000 0.39730(7) 0.0271(4) Uani 1 2 d S T P
Co1 Co 0.3833(4) 0.000000 0.1169(5) 0.0232(13) Uani 0.5 2 d S T P
Si1A Si 0.3833(4) 0.000000 0.1169(5) 0.0232(13) Uani 0.5 2 d S T P
Co2 Co 0.0197(5) 0.500000 0.2854(5) 0.0190(12) Uani 0.5 2 d S T P
Si2A Si 0.0197(5) 0.500000 0.2854(5) 0.0190(12) Uani 0.5 2 d S T P
Si1 Si 0.0131(7) 0.000000 0.1112(8) 0.0165(16) Uani 1 2 d S T P
Si2 Si 0.3877(8) 0.500000 0.2958(7) 0.0167(16) Uani 1 2 d S T P
O1 O -0.0415(17) 0.243(3) 0.1831(14) 0.044(4) Uani 1 1 d . . .
O2 O 0.4566(17) 0.263(3) 0.2149(14) 0.042(4) Uani 1 1 d . . .
O3 O 0.1779(9) 0.000000 0.0670(12) 0.033(2) Uani 1 2 d S T P
O4 O -0.0989(10) 0.000000 -0.0349(9) 0.047(3) Uani 1 2 d S T P
O5 O -0.0290(18) 0.456(4) 0.4239(10) 0.038(6) Uani 0.5 1 d . . P
O6 O 0.2059(9) 0.500000 0.2546(11) 0.0262(19) Uani 1 2 d S T P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Cs1 O2 47.9(6) 3_445 4_455
O2 Cs1 O1 111.5(4) 3_445 4
O2 Cs1 O1 90.6(4) 4_455 4
O2 Cs1 O1 90.6(4) 3_445 3_545
O2 Cs1 O1 111.5(4) 4_455 3_545
O1 Cs1 O1 52.1(7) 4 3_545
O2 Cs1 O5 92.8(4) 3_445 .
O2 Cs1 O5 55.3(3) 4_455 .
O1 Cs1 O5 103.4(5) 4 .
O1 Cs1 O5 154.4(4) 3_545 .
O2 Cs1 O5 55.3(3) 3_445 2
O2 Cs1 O5 92.8(4) 4_455 2
O1 Cs1 O5 154.4(4) 4 2
O1 Cs1 O5 103.4(5) 3_545 2
O5 Cs1 O5 99.3(7) . 2
O2 Cs1 O4 142.2(3) 3_445 3
O2 Cs1 O4 97.4(4) 4_455 3
O1 Cs1 O4 44.5(3) 4 3
O1 Cs1 O4 90.2(4) 3_545 3
O5 Cs1 O4 71.9(3) . 3
O5 Cs1 O4 158.7(3) 2 3
O2 Cs1 O4 97.4(3) 3_445 3_545
O2 Cs1 O4 142.2(3) 4_455 3_545
O1 Cs1 O4 90.2(4) 4 3_545
O1 Cs1 O4 44.5(3) 3_545 3_545
O5 Cs1 O4 158.7(3) . 3_545
O5 Cs1 O4 71.9(3) 2 3_545
O4 Cs1 O4 109.2(2) 3 3_545
O2 Cs1 O6 137.9(3) 3_445 .
O2 Cs1 O6 97.6(3) 4_455 .
O1 Cs1 O6 88.1(3) 4 .
O1 Cs1 O6 128.9(4) 3_545 .
O5 Cs1 O6 45.5(2) . .
O5 Cs1 O6 116.5(3) 2 .
O4 Cs1 O6 43.7(2) 3 .
O4 Cs1 O6 120.23(17) 3_545 .
O2 Cs1 O6 97.6(3) 3_445 1_545
O2 Cs1 O6 137.9(3) 4_455 1_545
O1 Cs1 O6 128.9(4) 4 1_545
O1 Cs1 O6 88.1(3) 3_545 1_545
O5 Cs1 O6 116.5(3) . 1_545
O5 Cs1 O6 45.5(2) 2 1_545
O4 Cs1 O6 120.23(17) 3 1_545
O4 Cs1 O6 43.7(2) 3_545 1_545
O6 Cs1 O6 97.6(2) . 1_545
O2 Cs1 O5 55.7(3) 3_445 1_545
O2 Cs1 O5 95.6(4) 4_455 1_545
O1 Cs1 O5 150.0(4) 4 1_545
O1 Cs1 O5 98.6(5) 3_545 1_545
O5 Cs1 O5 104.2(4) . 1_545
O5 Cs1 O5 4.9(5) 2 1_545
O4 Cs1 O5 160.4(2) 3 1_545
O4 Cs1 O5 67.3(3) 3_545 1_545
O6 Cs1 O5 119.9(2) . 1_545
O6 Cs1 O5 43.4(2) 1_545 1_545
O2 Cs1 O5 95.6(4) 3_445 2_565
O2 Cs1 O5 55.7(3) 4_455 2_565
O1 Cs1 O5 98.6(5) 4 2_565
O1 Cs1 O5 150.0(4) 3_545 2_565
O5 Cs1 O5 4.9(5) . 2_565
O5 Cs1 O5 104.2(4) 2 2_565
O4 Cs1 O5 67.3(3) 3 2_565
O4 Cs1 O5 160.4(2) 3_545 2_565
O6 Cs1 O5 43.4(2) . 2_565
O6 Cs1 O5 119.9(2) 1_545 2_565
O5 Cs1 O5 109.1(6) 1_545 2_565
O3 Cs2 O3 118.1(3) 3 3_545
O3 Cs2 O2 78.4(3) 3 .
O3 Cs2 O2 124.9(3) 3_545 .
O3 Cs2 O2 124.9(3) 3 2
O3 Cs2 O2 78.4(3) 3_545 2
O2 Cs2 O2 53.6(6) . 2
O3 Cs2 O1 92.3(3) 3 1_655
O3 Cs2 O1 136.9(3) 3_545 1_655
O2 Cs2 O1 88.7(4) . 1_655
O2 Cs2 O1 109.9(4) 2 1_655
O3 Cs2 O1 136.9(3) 3 2_655
O3 Cs2 O1 92.3(3) 3_545 2_655
O2 Cs2 O1 109.9(4) . 2_655
O2 Cs2 O1 88.7(4) 2 2_655
O1 Cs2 O1 47.4(6) 1_655 2_655
O3 Cs2 O6 59.61(19) 3 3_545
O3 Cs2 O6 59.61(19) 3_545 3_545
O2 Cs2 O6 120.0(3) . 3_545
O2 Cs2 O6 120.0(3) 2 3_545
O1 Cs2 O6 130.1(3) 1_655 3_545
O1 Cs2 O6 130.1(3) 2_655 3_545
O3 Cs2 O5 54.1(3) 3 1_655
O3 Cs2 O5 132.1(3) 3_545 1_655
O2 Cs2 O5 101.0(4) . 1_655
O2 Cs2 O5 148.4(3) 2 1_655
O1 Cs2 O5 44.6(3) 1_655 1_655
O1 Cs2 O5 83.0(4) 2_655 1_655
O6 Cs2 O5 87.77(18) 3_545 1_655
O3 Cs2 O5 132.1(3) 3 2_655
O3 Cs2 O5 54.1(3) 3_545 2_655
O2 Cs2 O5 148.4(3) . 2_655
O2 Cs2 O5 101.0(4) 2 2_655
O1 Cs2 O5 83.0(4) 1_655 2_655
O1 Cs2 O5 44.6(3) 2_655 2_655
O6 Cs2 O5 87.77(18) 3_545 2_655
O5 Cs2 O5 94.2(7) 1_655 2_655
O3 Cs2 Co1 30.59(17) 3 3
O3 Cs2 Co1 113.4(2) 3_545 3
O2 Cs2 Co1 104.3(3) . 3
O2 Cs2 Co1 155.3(3) 2 3
O1 Cs2 Co1 77.0(3) 1_655 3
O1 Cs2 Co1 111.4(3) 2_655 3
O6 Cs2 Co1 57.75(10) 3_545 3
O5 Cs2 Co1 32.43(19) 1_655 3
O5 Cs2 Co1 103.4(3) 2_655 3
O3 Cs2 Co1 113.4(2) 3 3_545
O3 Cs2 Co1 30.59(17) 3_545 3_545
O2 Cs2 Co1 155.3(3) . 3_545
O2 Cs2 Co1 104.3(3) 2 3_545
O1 Cs2 Co1 111.4(3) 1_655 3_545
O1 Cs2 Co1 77.0(3) 2_655 3_545
O6 Cs2 Co1 57.75(10) 3_545 3_545
O5 Cs2 Co1 103.4(3) 1_655 3_545
O5 Cs2 Co1 32.43(19) 2_655 3_545
Co1 Cs2 Co1 94.41(11) 3 3_545
O3 Cs2 O5 50.4(3) 3 2_665
O3 Cs2 O5 135.6(3) 3_545 2_665
O2 Cs2 O5 96.6(4) . 2_665
O2 Cs2 O5 145.8(3) 2 2_665
O1 Cs2 O5 46.1(3) 1_655 2_665
O1 Cs2 O5 86.6(4) 2_655 2_665
O6 Cs2 O5 87.98(17) 3_545 2_665
O5 Cs2 O5 5.0(5) 1_655 2_665
O5 Cs2 O5 99.2(4) 2_655 2_665
Co1 Cs2 O5 31.18(15) 3 2_665
Co1 Cs2 O5 107.6(3) 3_545 2_665
O2 Co1 O2 104.3(11) 2 .
O2 Co1 O3 117.5(5) 2 .
O2 Co1 O3 117.5(5) . .
O2 Co1 O5 102.5(8) 2 3_544
O2 Co1 O5 113.8(8) . 3_544
O3 Co1 O5 100.4(6) . 3_544
O2 Co1 O5 113.8(8) 2 4_554
O2 Co1 O5 102.5(8) . 4_554
O3 Co1 O5 100.4(6) . 4_554
O5 Co1 O5 13.6(12) 3_544 4_554
O2 Co1 Cs2 80.6(5) 2 3_444
O2 Co1 Cs2 175.0(5) . 3_444
O3 Co1 Cs2 58.82(19) . 3_444
O5 Co1 Cs2 65.0(6) 3_544 3_444
O5 Co1 Cs2 75.6(6) 4_554 3_444
O2 Co1 Cs2 175.0(5) 2 3_454
O2 Co1 Cs2 80.6(5) . 3_454
O3 Co1 Cs2 58.82(19) . 3_454
O5 Co1 Cs2 75.6(6) 3_544 3_454
O5 Co1 Cs2 65.0(6) 4_554 3_454
Cs2 Co1 Cs2 94.41(11) 3_444 3_454
O2 Co1 Cs2 53.3(5) 2 .
O2 Co1 Cs2 53.3(5) . .
O3 Co1 Cs2 152.1(4) . .
O5 Co1 Cs2 107.2(5) 3_544 .
O5 Co1 Cs2 107.2(5) 4_554 .
Cs2 Co1 Cs2 131.55(5) 3_444 .
Cs2 Co1 Cs2 131.55(5) 3_454 .
O2 Co1 Cs1 114.8(5) 2 3_554
O2 Co1 Cs1 49.7(5) . 3_554
O3 Co1 Cs1 127.5(2) . 3_554
O5 Co1 Cs1 64.1(6) 3_544 3_554
O5 Co1 Cs1 53.4(6) 4_554 3_554
Cs2 Co1 Cs1 128.89(14) 3_444 3_554
Cs2 Co1 Cs1 68.68(5) 3_454 3_554
Cs2 Co1 Cs1 69.90(6) . 3_554
O2 Co1 Cs1 49.7(5) 2 3_544
O2 Co1 Cs1 114.8(5) . 3_544
O3 Co1 Cs1 127.5(2) . 3_544
O5 Co1 Cs1 53.4(6) 3_544 3_544
O5 Co1 Cs1 64.1(6) 4_554 3_544
Cs2 Co1 Cs1 68.68(5) 3_444 3_544
Cs2 Co1 Cs1 128.89(14) 3_454 3_544
Cs2 Co1 Cs1 69.90(6) . 3_544
Cs1 Co1 Cs1 84.99(8) 3_554 3_544
O2 Co1 Cs1 72.7(5) 2 .
O2 Co1 Cs1 72.7(5) . .
O3 Co1 Cs1 77.9(4) . .
O5 Co1 Cs1 173.0(6) 3_544 .
O5 Co1 Cs1 173.0(6) 4_554 .
Cs2 Co1 Cs1 108.76(8) 3_444 .
Cs2 Co1 Cs1 108.76(8) 3_454 .
Cs2 Co1 Cs1 74.23(9) . .
Cs1 Co1 Cs1 122.31(9) 3_554 .
Cs1 Co1 Cs1 122.31(9) 3_544 .
O5 Co2 O5 19.6(18) 2_565 .
O5 Co2 O6 119.3(8) 2_565 .
O5 Co2 O6 119.3(8) . .
O5 Co2 O1 122.3(10) 2_565 .
O5 Co2 O1 105.4(11) . .
O6 Co2 O1 101.4(6) . .
O5 Co2 O1 105.4(11) 2_565 2_565
O5 Co2 O1 122.3(10) . 2_565
O6 Co2 O1 101.4(6) . 2_565
O1 Co2 O1 104.2(10) . 2_565
O5 Co2 Cs1 75.0(8) 2_565 .
O5 Co2 Cs1 59.5(8) . .
O6 Co2 Cs1 72.8(2) . .
O1 Co2 Cs1 81.0(5) . .
O1 Co2 Cs1 173.1(5) 2_565 .
O5 Co2 Cs1 59.5(8) 2_565 1_565
O5 Co2 Cs1 75.0(8) . 1_565
O6 Co2 Cs1 72.8(2) . 1_565
O1 Co2 Cs1 173.1(5) . 1_565
O1 Co2 Cs1 81.0(5) 2_565 1_565
Cs1 Co2 Cs1 93.52(9) . 1_565
O5 Co2 Cs1 111.7(7) 2_565 3_454
O5 Co2 Cs1 111.7(7) . 3_454
O6 Co2 Cs1 128.1(4) . 3_454
O1 Co2 Cs1 54.6(5) . 3_454
O1 Co2 Cs1 54.6(5) 2_565 3_454
Cs1 Co2 Cs1 131.98(5) . 3_454
Cs1 Co2 Cs1 131.98(5) 1_565 3_454
O5 Co2 Cs2 69.0(8) 2_565 1_455
O5 Co2 Cs2 53.9(8) . 1_455
O6 Co2 Cs2 136.25(9) . 1_455
O1 Co2 Cs2 53.4(6) . 1_455
O1 Co2 Cs2 118.2(5) 2_565 1_455
Cs1 Co2 Cs2 68.54(5) . 1_455
Cs1 Co2 Cs2 128.36(13) 1_565 1_455
Cs1 Co2 Cs2 70.39(7) 3_454 1_455
O5 Co2 Cs2 53.9(8) 2_565 1_465
O5 Co2 Cs2 69.0(8) . 1_465
O6 Co2 Cs2 136.25(9) . 1_465
O1 Co2 Cs2 118.2(5) . 1_465
O1 Co2 Cs2 53.4(6) 2_565 1_465
Cs1 Co2 Cs2 128.36(13) . 1_465
Cs1 Co2 Cs2 68.54(5) 1_565 1_465
Cs1 Co2 Cs2 70.39(7) 3_454 1_465
Cs2 Co2 Cs2 85.23(9) 1_455 1_465
O5 Co2 Cs2 168.0(8) 2_565 3_454
O5 Co2 Cs2 168.0(8) . 3_454
O6 Co2 Cs2 53.3(4) . 3_454
O1 Co2 Cs2 69.7(6) . 3_454
O1 Co2 Cs2 69.7(6) 2_565 3_454
Cs1 Co2 Cs2 108.55(9) . 3_454
Cs1 Co2 Cs2 108.55(9) 1_565 3_454
Cs1 Co2 Cs2 74.82(8) 3_454 3_454
Cs2 Co2 Cs2 122.97(8) 1_455 3_454
Cs2 Co2 Cs2 122.97(8) 1_465 3_454
O3 Si1 O1 115.3(7) . 2
O3 Si1 O1 115.3(7) . .
O1 Si1 O1 114.9(13) 2 .
O3 Si1 O4 109.7(7) . .
O1 Si1 O4 99.4(6) 2 .
O1 Si1 O4 99.4(6) . .
O3 Si1 Cs2 151.3(6) . 1_455
O1 Si1 Cs2 57.9(7) 2 1_455
O1 Si1 Cs2 57.9(7) . 1_455
O4 Si1 Cs2 99.0(4) . 1_455
O3 Si1 Cs2 52.8(2) . 3_444
O1 Si1 Cs2 77.6(7) 2 3_444
O1 Si1 Cs2 166.9(7) . 3_444
O4 Si1 Cs2 81.6(3) . 3_444
Cs2 Si1 Cs2 135.06(7) 1_455 3_444
O3 Si1 Cs2 52.8(2) . 3_454
O1 Si1 Cs2 166.9(7) 2 3_454
O1 Si1 Cs2 77.6(7) . 3_454
O4 Si1 Cs2 81.6(3) . 3_454
Cs2 Si1 Cs2 135.06(7) 1_455 3_454
Cs2 Si1 Cs2 89.74(15) 3_444 3_454
O3 Si1 Cs1 83.6(5) . .
O1 Si1 Cs1 73.9(5) 2 .
O1 Si1 Cs1 73.9(5) . .
O4 Si1 Cs1 166.7(4) . .
Cs2 Si1 Cs1 67.70(12) 1_455 .
Cs2 Si1 Cs1 107.56(11) 3_444 .
Cs2 Si1 Cs1 107.56(11) 3_454 .
O3 Si1 Cs1 127.9(3) . 3_444
O1 Si1 Cs1 46.3(5) 2 3_444
O1 Si1 Cs1 116.0(7) . 3_444
O4 Si1 Cs1 53.16(19) . 3_444
Cs2 Si1 Cs1 70.22(10) 1_455 3_444
Cs2 Si1 Cs1 75.11(6) 3_444 3_444
Cs2 Si1 Cs1 133.52(19) 3_454 3_444
Cs1 Si1 Cs1 118.87(14) . 3_444
O3 Si1 Cs1 127.9(3) . 3_454
O1 Si1 Cs1 116.0(7) 2 3_454
O1 Si1 Cs1 46.3(5) . 3_454
O4 Si1 Cs1 53.16(19) . 3_454
Cs2 Si1 Cs1 70.22(10) 1_455 3_454
Cs2 Si1 Cs1 133.52(19) 3_444 3_454
Cs2 Si1 Cs1 75.11(6) 3_454 3_454
Cs1 Si1 Cs1 118.87(14) . 3_454
Cs1 Si1 Cs1 84.14(11) 3_444 3_454
O4 Si2 O2 116.5(6) 3 .
O4 Si2 O2 116.5(6) 3 2_565
O2 Si2 O2 104.8(12) . 2_565
O4 Si2 O6 106.1(6) 3 .
O2 Si2 O6 105.9(6) . .
O2 Si2 O6 105.9(6) 2_565 .
O4 Si2 Cs1 60.2(2) 3 .
O2 Si2 Cs1 82.3(6) . .
O2 Si2 Cs1 172.7(6) 2_565 .
O6 Si2 Cs1 70.1(3) . .
O4 Si2 Cs1 60.2(2) 3 1_565
O2 Si2 Cs1 172.7(6) . 1_565
O2 Si2 Cs1 82.3(6) 2_565 1_565
O6 Si2 Cs1 70.1(3) . 1_565
Cs1 Si2 Cs1 90.62(15) . 1_565
O4 Si2 Cs1 131.1(5) 3 3_554
O2 Si2 Cs1 52.7(6) . 3_554
O2 Si2 Cs1 52.7(6) 2_565 3_554
O6 Si2 Cs1 122.7(4) . 3_554
Cs1 Si2 Cs1 134.57(8) . 3_554
Cs1 Si2 Cs1 134.57(8) 1_565 3_554
O4 Si2 Cs2 161.5(5) 3 3_454
O2 Si2 Cs2 73.0(6) . 3_454
O2 Si2 Cs2 73.0(6) 2_565 3_454
O6 Si2 Cs2 55.4(4) . 3_454
Cs1 Si2 Cs2 108.22(13) . 3_454
Cs1 Si2 Cs2 108.22(13) 1_565 3_454
Cs1 Si2 Cs2 67.34(11) 3_554 3_454
O4 Si2 Cs2 74.6(3) 3 .
O2 Si2 Cs2 45.7(6) . .
O2 Si2 Cs2 110.9(6) 2_565 .
O6 Si2 Cs2 138.08(8) . .
Cs1 Si2 Cs2 75.08(6) . .
Cs1 Si2 Cs2 133.51(17) 1_565 .
Cs1 Si2 Cs2 69.50(11) 3_554 .
Cs2 Si2 Cs2 118.26(13) 3_454 .
O4 Si2 Cs2 74.6(3) 3 1_565
O2 Si2 Cs2 110.9(6) . 1_565
O2 Si2 Cs2 45.7(6) 2_565 1_565
O6 Si2 Cs2 138.08(8) . 1_565
Cs1 Si2 Cs2 133.51(17) . 1_565
Cs1 Si2 Cs2 75.08(6) 1_565 1_565
Cs1 Si2 Cs2 69.50(11) 3_554 1_565
Cs2 Si2 Cs2 118.26(13) 3_454 1_565
Cs2 Si2 Cs2 83.41(13) . 1_565
Si1 O1 Co2 143.2(10) . .
Si1 O1 Cs1 112.9(7) . 3_454
Co2 O1 Cs1 98.5(7) . 3_454
Si1 O1 Cs2 98.3(9) . 1_455
Co2 O1 Cs2 100.9(6) . 1_455
Cs1 O1 Cs2 89.3(4) 3_454 1_455
Si2 O2 Co1 136.4(10) . .
Si2 O2 Cs1 103.3(8) . 3_554
Co1 O2 Cs1 104.4(6) . 3_554
Si2 O2 Cs2 112.8(7) . .
Co1 O2 Cs2 99.4(7) . .
Cs1 O2 Cs2 91.5(4) 3_554 .
Si1 O3 Co1 150.1(8) . .
Si1 O3 Cs2 104.3(3) . 3_444
Co1 O3 Cs2 90.6(2) . 3_444
Si1 O3 Cs2 104.3(3) . 3_454
Co1 O3 Cs2 90.6(2) . 3_454
Cs2 O3 Cs2 118.1(3) 3_444 3_454
Si2 O4 Si1 147.5(8) 3_444 .
Si2 O4 Cs1 95.4(3) 3_444 3_444
Si1 O4 Cs1 103.2(3) . 3_444
Si2 O4 Cs1 95.4(3) 3_444 3_454
Si1 O4 Cs1 103.2(3) . 3_454
Cs1 O4 Cs1 109.2(2) 3_444 3_454
O5 O5 Co2 80.2(9) 2_565 .
O5 O5 Co1 83.2(6) 2_565 3_455
Co2 O5 Co1 162.7(15) . 3_455
O5 O5 Cs1 139.7(3) 2_565 .
Co2 O5 Cs1 98.7(9) . .
Co1 O5 Cs1 97.0(6) 3_455 .
O5 O5 Cs2 137.1(3) 2_565 1_455
Co2 O5 Cs2 106.6(9) . 1_455
Co1 O5 Cs2 82.6(5) 3_455 1_455
Cs1 O5 Cs2 82.3(5) . 1_455
O5 O5 Cs1 35.5(3) 2_565 1_565
Co2 O5 Cs1 83.2(8) . 1_565
Co1 O5 Cs1 86.1(6) 3_455 1_565
Cs1 O5 Cs1 104.2(4) . 1_565
Cs2 O5 Cs1 167.6(4) 1_455 1_565
O5 O5 Cs2 37.9(3) 2_565 1_465
Co2 O5 Cs2 90.6(9) . 1_465
Co1 O5 Cs2 73.2(6) 3_455 1_465
Cs1 O5 Cs2 169.8(3) . 1_465
Cs2 O5 Cs2 99.2(4) 1_455 1_465
Cs1 O5 Cs2 72.6(4) 1_565 1_465
Si2 O6 Co2 156.8(7) . .
Si2 O6 Cs2 100.5(4) . 3_454
Co2 O6 Cs2 102.7(4) . 3_454
Si2 O6 Cs1 84.3(3) . .
Co2 O6 Cs1 80.5(3) . .
Cs2 O6 Cs1 131.18(12) 3_454 .
Si2 O6 Cs1 84.3(3) . 1_565
Co2 O6 Cs1 80.5(3) . 1_565
Cs2 O6 Cs1 131.18(12) 3_454 1_565
Cs1 O6 Cs1 97.6(2) . 1_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cs1 O2 3.182(16) 3_445
Cs1 O2 3.182(16) 4_455
Cs1 O1 3.197(14) 4
Cs1 O1 3.197(14) 3_545
Cs1 O5 3.27(2) .
Cs1 O5 3.27(2) 2
Cs1 O4 3.349(5) 3
Cs1 O4 3.349(5) 3_545
Cs1 O6 3.628(7) .
Cs1 O6 3.628(7) 1_545
Cs1 O5 3.65(2) 1_545
Cs1 O5 3.65(2) 2_565
Cs2 O3 3.183(6) 3
Cs2 O3 3.183(6) 3_545
Cs2 O2 3.187(16) .
Cs2 O2 3.187(16) 2
Cs2 O1 3.297(18) 1_655
Cs2 O1 3.297(18) 2_655
Cs2 O6 3.360(10) 3_545
Cs2 O5 3.40(2) 1_655
Cs2 O5 3.40(2) 2_655
Cs2 Co1 3.720(3) 3
Cs2 Co1 3.720(3) 3_545
Cs2 O5 3.76(2) 2_665
Co1 O2 1.821(16) 2
Co1 O2 1.821(16) .
Co1 O3 1.893(10) .
Co1 O5 2.012(11) 3_544
Co1 O5 2.012(11) 4_554
Co2 O5 1.405(10) 2_565
Co2 O5 1.405(10) .
Co2 O6 1.707(10) .
Co2 O1 1.781(17) .
Co2 O1 1.781(17) 2_565
Si1 O3 1.550(10) .
Si1 O1 1.572(17) 2
Si1 O1 1.572(17) .
Si1 O4 1.680(12) .
Si2 O4 1.592(11) 3
Si2 O2 1.630(16) .
Si2 O2 1.630(16) 2_565
Si2 O6 1.670(11) .
O5 O5 0.48(4) 2_565
